CHAPTER 14
POLYMER STRUCTURES
PROBLEM SOLUTIONS
Hydrocarbon Molecules
Polymer Molecules
The Chemistry of Polymer Molecules
14.1 On the basis of the structures presented in this chapter, sketch repeat unit structures for the following polymers: (a) polychlorotrifluoroethylene, and (b) poly(vinyl alcohol).
Solution
The repeat unit structures called for are sketched below.
(a) Polychlorotrifluoroethylene
(b) Poly(vinyl alcohol)
Molecular Weight
14.2 Compute repeat unit molecular weights for the following: (a) poly(vinyl chloride), (b) poly(ethylene terephthalate), (c) polycarbonate, and (d) polydimethylsiloxane.
Solution
(a) For poly(vinyl chloride), each repeat unit consists of two carbons, three hydrogens, and one chlorine (Table 14.3). If A_{C}, A_{H} and A_{Cl} represent the atomic weights of carbon, hydrogen, and chlorine, respectively, then
m = 2(A_{C}) + 3(A_{H}) + (A_{Cl})
= (2)(12.01 g/mol) + (3)(1.008 g/mol) + 35.45 g/mol = 62.49 g/mol
(b) For poly(ethylene terephthalate), from Table 14.3, each repeat unit has ten carbons, eight hydrogens, and four oxygens. Thus,
m = 10(A_{C}) + 8(A_{H}) + 4(A_{O})
= (10)(12.01 g/mol) + (8)(1.008 g/mol) + (4)(16.00 g/mol) = 192.16 g/mol
(c) For polycarbonate, from Table 14.3, each repeat unit has sixteen carbons, fourteen hydrogens, and three oxygens. Thus,
m = 16(A_{C}) + 14(A_{H}) + 3(A_{O})
= (16)(12.01 g/mol) + (14)(1.008 g/mol) + (3)(16.00 g/mol)
= 254.27 g/mol
(d) For polydimethylsiloxane, from Table 14.5, each repeat unit has two carbons, six hydrogens, one silicon and one oxygen. Thus,
m = 2(A_{C}) + 6(A_{H}) + (A_{Si}) + (A_{O})
= (2)(12.01 g/mol) + (6)(1.008 g/mol) + (28.09 g/mol) + (16.00 g/mol) = 74.16 g/mol
14.3 The numberaverage molecular weight of a polypropylene is 1,000,000 g/mol. Compute the degree of polymerization.
Solution
We are asked to compute the degree of polymerization for polypropylene, given that the numberaverage molecular weight is 1,000,000 g/mol. The repeat unit molecular weight of polypropylene is just
m = 3(A_{C}) + 6(A_{H})
= (3)(12.01 g/mol) + (6)(1.008 g/mol) = 42.08 g/mol
Now it is possible to compute the degree of polymerization using Equation 14.6 as
14.4 (a) Compute the repeat unit molecular weight of polystyrene.
(b) Compute the numberaverage molecular weight for a polystyrene for which the degree of polymerization is 25,000.
Solution
(a) The repeat unit molecular weight of polystyrene is called for in this portion of the problem. For polystyrene, from Table 14.3, each repeat unit has eight carbons and eight hydrogens. Thus,
m = 8(A_{C}) + 8(A_{H})
= (8)(12.01 g/mol) + (8)(1.008 g/mol) = 104.14 g/mol
(b) We are now asked to compute the numberaverage molecular weight. Since the degree of polymerization is 25,000, using Equation 14.6
14.5 Below, molecular weight data for a polypropylene material are tabulated. Compute (a) the numberaverage molecular weight, (b) the weightaverage molecular weight, and (c) the degree of polymerization.
Molecular Weight
Range (g/mol)

x_{i}

w_{i}

8,000–16,000

0.05

0.02

16,000–24,000

0.16

0.10

24,000–32,000

0.24

0.20

32,000–40,000

0.28

0.30

40,000–48,000

0.20

0.27

48,000–56,000

0.07

0.11

Solution
(a) From the tabulated data, we are asked to compute , the numberaverage molecular weight. This is carried out below.
Molecular wt
Range Mean M_{i} x_{i} x_{i}M_{i}
8,00016,000 12,000 0.05 600
16,00024,000 20,000 0.16 3200
24,00032,000 28,000 0.24 6720
32,00040,000 36,000 0.28 10,080
40,00048,000 44,000 0.20 8800
48,00056,000 52,000 0.07 3640
____________________________
^{ }
(b) From the tabulated data, we are asked to compute , the weightaverage molecular weight.
Molecular wt.
Range Mean M_{i} w_{i} w_{i}M_{i}
8,00016,000 12,000 0.02 240
16,00024,000 20,000 0.10 2000
24,00032,000 28,000 0.20 5600
32,00040,000 36,000 0.30 10,800
40,00048,000 44,000 0.27 11,880
48,00056,000 52,000 0.11 5720
___________________________
^{ }
(c) Now we are asked to compute the degree of polymerization, which is possible using Equation 14.6. For polypropylene, the repeat unit molecular weight is just
m = 3(A_{C}) + 6(A_{H})
= (3)(12.01 g/mol) + (6)(1.008 g/mol) = 42.08 g/mol
And
14.6 Molecular weight data for some polymer are tabulated here. Compute (a) the numberaverage molecular weight, and (b) the weightaverage molecular weight. (c) If it is known that this material's degree of polymerization is 710, which one of the polymers listed in Table 14.3 is this polymer? Why?
Molecular Weight
Range g/mol

x_{i}

w_{i}

15,000–30,000

0.04

0.01

30,000–45,000

0.07

0.04

45,000–60,000

0.16

0.11

60,000–75,000

0.26

0.24

75,000–90,000

0.24

0.27

90,000–105,000

0.12

0.16

105,000–120,000

0.08

0.12

120,000–135,000

0.03

0.05

Solution
(a) From the tabulated data, we are asked to compute , the numberaverage molecular weight. This is carried out below.
Molecular wt.
Range Mean M_{i} x_{i} x_{i}M_{i}
15,00030,000 22,500 0.04 900
30,00045,000 37,500 0.07 2625
45,00060,000 52,500 0.16 8400
60,00075,000 67,500 0.26 17,550
75,00090,000 82,500 0.24 19,800
90,000105,000 97,500 0.12 11,700
105,000120,000 112,500 0.08 9000
120,000135,000 127,500 0.03 3825
_________________________^{ }
(b) From the tabulated data, we are asked to compute , the weightaverage molecular weight. This determination is performed as follows:
Molecular wt.
Range Mean M_{i} w_{i} w_{i}M_{i}
15,00030,000 22,500 0.01 225
30,00045,000 37,500 0.04 1500
45,00060,000 52,500 0.11 5775
60,00075,000 67,500 0.24 16,200
75,00090,000 82,500 0.27 22,275
90,000105,000 97,500 0.16 15,600
105,000120,000 112,500 0.12 13,500
120,000135,000 127,500 0.05 6375
_________________________
^{ }
(c) We are now asked if the degree of polymerization is 710, which of the polymers in Table 14.3 is this material? It is necessary to compute m in Equation 14.6 as
The repeat unit molecular weights of the polymers listed in Table 14.3 are as follows:
Polyethylene28.05 g/mol
Poly(vinyl chloride)62.49 g/mol
Polytetrafluoroethylene100.02 g/mol
Polypropylene42.08 g/mol
Polystyrene104.14 g/mol
Poly(methyl methacrylate)100.11 g/mol
Phenolformaldehyde133.16 g/mol
Nylon 6,6226.32 g/mol
PET192.16 g/mol
Polycarbonate254.27 g/mol
Therefore, polystyrene is the material since its repeat unit molecular weight is closest to that calculated above.
14.7 Is it possible to have a poly(methyl methacrylate) homopolymer with the following molecular weight data and a of polymerization of 527? Why or why not?
Molecular Weight
Range (g/mol)

w_{i}

x_{i}

8,000–20,000

0.02

0.05

20,000–32,000

0.08

0.15

32,000–44,000

0.17

0.21

44,000–56,000

0.29

0.28

56,000–68,000

0.23

0.18

68,000–80,000

0.16

0.10

80,000–92,000

0.05

0.03

Solution
This problem asks if it is possible to have a poly(methyl methacrylate) homopolymer with the given molecular weight data and a degree of polymerization of 527. The appropriate data are given below along with a computation of the numberaverage molecular weight.
Molecular wt.
Range Mean M_{i} x_{i} x_{i}M_{i}
8,00020,000 14,000 0.05 700
20,00032,000 26,000 0.15 3900
32,00044,000 38,000 0.21 7980
44,00056,000 50,000 0.28 14,000
56,00068,000 62,000 0.18 11,160
68,00080,000 74,000 0.10 7400
80,00092,000 86,000 0.03 2580
_________________________
^{ }
For PMMA, from Table 14.3, each repeat unit has five carbons, eight hydrogens, and two oxygens. Thus,
m = 5(A_{C}) + 8(A_{H}) + 2(A_{O})
= (5)(12.01 g/mol) + (8)(1.008 g/mol) + (2)(16.00 g/mol) = 100.11 g/mol
Now, we will compute the degree of polymerization using Equation 14.6 as
Thus, such a homopolymer is not possible since the calculated degree of polymerization is 477 (and not 527).
14.8 Highdensity polyethylene may be chlorinated by inducing the random substitution of chlorine atoms for hydrogen.
(a) Determine the concentration of Cl (in wt%) that must be added if this substitution occurs for 5% of all the original hydrogen atoms.
(b) In what ways does this chlorinated polyethylene differ from poly(vinyl chloride)?
Solution
(a) For chlorinated polyethylene, we are asked to determine the weight percent of chlorine added for 5% Cl substitution of all original hydrogen atoms. Consider 50 carbon atoms; there are 100 possible sidebonding sites. Ninetyfive are occupied by hydrogen and five are occupied by Cl. Thus, the mass of these 50 carbon atoms, m_{C}, is just
m_{C} = 50(A_{C}) = (50)(12.01 g/mol) = 600.5 g
Likewise, for hydrogen and chlorine,
m_{H} = 95(A_{H}) = (95)(1.008 g/mol) = 95.76 g
m_{Cl} = 5(A_{Cl}) = (5)(35.45 g/mol) = 177.25 g
Thus, the concentration of chlorine, C_{Cl}, is determined using a modified form of Equation 4.3 as
(b) Chlorinated polyethylene differs from poly(vinyl chloride), in that, for PVC, (1) 25% of the sidebonding sites are substituted with Cl, and (2) the substitution is probably much less random.
Molecular Shape
14.9 For a linear polymer molecule, the total chain length L depends on the bond length between chain atoms d, the total number of bonds in the molecule N, and the angle between adjacent backbone chain atoms θ, as follows:
(14.11)
Furthermore, the average endtoend distance for a series of polymer molecules r in Figure 14.6 is equal to
(14.12)
A linear polytetrafluoroethylene has a numberaverage molecular weight of 500,000 g/mol; compute average values of L and r for this material.
Solution
This problem first of all asks for us to calculate, using Equation 14.11, the average total chain length, L, for a linear polytetrafluoroethylene polymer having a numberaverage molecular weight of 500,000 g/mol. It is necessary to calculate the degree of polymerization, DP, using Equation 14.6. For polytetrafluoroethylene, from Table 14.3, each repeat unit has two carbons and four flourines. Thus,
m = 2(A_{C}) + 4(A_{F})
= (2)(12.01 g/mol) + (4)(19.00 g/mol) = 100.02 g/mol
and
which is the number of repeat units along an average chain. Since there are two carbon atoms per repeat unit, there are two C—C chain bonds per repeat unit, which means that the total number of chain bonds in the molecule, N, is just (2)(5000) = 10,000 bonds. Furthermore, assume that for single carboncarbon bonds, d = 0.154 nm and = 109 (Section 14.4); therefore, from Equation 14.11
It is now possible to calculate the average chain endtoend distance, r, using Equation 14.12 as
14.10 Using the definitions for total chain molecule length, L (Equation 14.11) and average chain endtoend distance r (Equation 14.12), for a linear polyethylene determine:
(a) the numberaverage molecular weight for L = 2500 nm;
(b) the numberaverage molecular weight for r = 20 nm.
Solution
(a) This portion of the problem asks for us to calculate the numberaverage molecular weight for a linear polyethylene for which L in Equation 14.11 is 2500 nm. It is first necessary to compute the value of N using this equation, where, for the C—C chain bond, d = 0.154 nm, and = 109. Thus
Since there are two C—C bonds per polyethylene repeat unit, there is an average of N/2 or 19,940/2 = 9970 repeat units per chain, which is also the degree of polymerization, DP. In order to compute the value of using Equation 14.6, we must first determine m for polyethylene. Each polyethylene repeat unit consists of two carbon and four hydrogen atoms, thus
m = 2(A_{C}) + 4(A_{H})
= (2)(12.01 g/mol) + (4)(1.008 g/mol) = 28.05 g/mol
Therefore
(b) Next, we are to determine the numberaverage molecular weight for r = 20 nm. Solving for N from Equation 14.12 leads to
which is the total number of bonds per average molecule. Since there are two C—C bonds per repeat unit, then DP = N/2 = 16,900/2 = 8450. Now, from Equation 14.6
Molecular Configurations
14.11 Sketch portions of a linear polystyrene molecule that are (a) syndiotactic, (b) atactic, and (c) isotactic. Use twodimensional schematics per footnote 8 of this chapter.
Solution
We are asked to sketch portions of a linear polystyrene molecule for different configurations (using twodimensional schematic sketches).
(a) Syndiotactic polystyrene
(b) Atactic polystyrene
(c) Isotactic polystyrene
14.12 Sketch cis and trans structures for (a) butadiene, and (b) chloroprene. Use twodimensional schematics per footnote 11 of this chapter.
Solution
This problem asks for us to sketch cis and trans structures for butadiene and chloroprene.
(a) The structure for cis polybutadiene (Table 14.5) is
The structure of trans butadiene is
(b) The structure of cis chloroprene (Table 14.5) is
The structure of trans chloroprene is
Thermoplastic and Thermosetting Polymers
14.13 Make comparisons of thermoplastic and thermosetting polymers (a) on the basis of mechanical characteristics upon heating, and (b) according to possible molecular structures.
Solution
(a) Thermoplastic polymers soften when heated and harden when cooled, whereas thermosetting polymers, harden upon heating, while further heating will not lead to softening.
(b) Thermoplastic polymers have linear and branched structures, while for thermosetting polymers, the structures will normally be network or crosslinked.
14.14 (a) Is it possible to grind up and reuse phenolformaldehyde? Why or why not?
(b) Is it possible to grind up and reuse polypropylene? Why or why not?
Solution
(a) It is not possible to grind up and reuse phenolformaldehyde because it is a network thermoset polymer and, therefore, is not amenable to remolding.
(b) Yes, it is possible to grind up and reuse polypropylene since it is a thermoplastic polymer, will soften when reheated, and, thus, may be remolded.
Copolymers
14.15 Sketch the repeat structure for each of the following alternating copolymers: (a) poly(butadienechloroprene), (b) poly(styrenemethyl methacrylate), and (c) poly(acrylonitrilevinyl chloride).
Solution
This problem asks for sketches of the repeat unit structures for several alternating copolymers.
(a) For poly(butadienechloroprene)
(b) For poly(styrenemethyl methacrylate)
(c) For poly(acrylonitrilevinyl chloride)
14.16 The numberaverage molecular weight of a poly(styrenebutadiene) alternating copolymer is 1,350,000 g/mol; determine the average number of styrene and butadiene repeat units per molecule.
Solution
Since it is an alternating copolymer, the number of both types of repeat units will be the same. Therefore, consider them as a single repeat unit, and determine the numberaverage degree of polymerization. For the styrene repeat unit, there are eight carbon atoms and eight hydrogen atoms, while the butadiene repeat consists of four carbon atoms and six hydrogen atoms. Therefore, the styrenebutadiene combined repeat unit weight is just
m = 12(A_{C}) + 14(A_{H})
= (12)(12.01 g/mol) + (14)(1.008 g/mol) = 158.23 g/mol
From Equation 14.6, the degree of polymerization is just
Thus, there is an average of 8530 of both repeat unit types per molecule.
14.17 Calculate the numberaverage molecular weight of a random nitrile rubber [poly(acrylonitrilebutadiene) copolymer] in which the fraction of butadiene repeat units is 0.30; assume that this concentration corresponds to a degree of polymerization of 2000.
Solution
This problem asks for us to calculate the numberaverage molecular weight of a random nitrile rubber copolymer. For the acrylonitrile repeat unit there are three carbon, one nitrogen, and three hydrogen atoms. Thus, its repeat unit molecular weight is
m_{Ac} = 3(A_{C}) + (A_{N}) + 3(A_{H})
= (3)(12.01 g/mol) + 14.01 g/mol + (3)(1.008 g/mol) = 53.06 g/mol
The butadiene repeat unit is composed of four carbon and six hydrogen atoms. Thus, its repeat unit molecular weight is
m_{Bu} = 4(A_{C}) + 6(A_{H})
= (4)(12.01 g/mol) + (6)(1.008 g/mol) = 54.09 g/mol
From Equation 14.7, the average repeat unit molecular weight is just
= (0.70)(53.06 g/mol) + (0.30)(54.09 g/mol) = 53.37 g/mol
Since DP = 2000 (as stated in the problem), may be computed using Equation 14.6 as
14.18 An alternating copolymer is known to have a numberaverage molecular weight of 250,000 g/mol and a degree of polymerization of 3420. If one of the repeat units is styrene, which of ethylene, propylene, tetrafluoroethylene, and vinyl chloride is the other repeat unit? Why?
Solution
For an alternating copolymer which has a numberaverage molecular weight of 250,000 g/mol and a degree of polymerization of 3420, we are to determine one of the repeat unit types if the other is styrene. It is first necessary to calculate using Equation 14.6 as
Since this is an alternating copolymer we know that chain fraction of each repeat unit type is 0.5; that is f_{s} = f_{x} = 0.5, f_{s} and f_{x} being, respectively, the chain fractions of the styrene and unknown repeat units. Also, the repeat unit molecular weight for styrene is
m_{s} = 8(A_{C}) + 8(A_{H})
= 8(12.01 g/mol) + 8(1.008 g/mol) = 104.14 g/mol
Now, using Equation 14.7, it is possible to calculate the repeat unit weight of the unknown repeat unit type, m_{x}. Thus
Finally, it is necessary to calculate the repeat unit molecular weights for each of the possible other repeat unit types. These are calculated below:
m_{ethylene} = 2(A_{C}) + 4(A_{H}) = 2(12.01 g/mol) + 4(1.008 g/mol) = 28.05 g/mol
m_{propylene} = 3(A_{C}) + 6(A_{H}) = 3(12.01 g/mol) + 6(1.008 g/mol) = 42.08 g/mol
m_{TFE} = 2(A_{C}) + 4(A_{F}) = 2(12.01 g/mol) + 4(19.00 g/mol) = 100.02 g/mol
m_{VC} = 2(A_{C}) + 3(A_{H}) + (A_{Cl}) = 2(12.01 g/mol) + 3(1.008 g/mol) + 35.45 g/mol = 62.49 g/mol
Therefore, propylene is the other repeat unit type since its m value is almost the same as the calculated m_{x}.
14.19 (a) Determine the ratio of butadiene to styrene repeat units in a copolymer having a numberaverage molecular weight of 350,000 g/mol and degree of polymerization of 4425.
(b) Which type(s) of copolymer(s) will this copolymer be, considering the following possibilities: random, alternating, graft, and block? Why?
Solution
(a) This portion of the problem asks us to determine the ratio of butadiene to styrene repeat units in a copolymer having a weightaverage molecular weight of 350,000 g/mol and a degree of polymerization of 4425. It first becomes necessary to calculate the average repeat unit molecular weight of the copolymer, , using Equation 14.6 as
If we designate f_{b} as the chain fraction of butadiene repeat units, since the copolymer consists of only two repeat unit types, the chain fraction of styrene repeat units f_{s} is just 1 – f_{b}. Now, Equation 14.7 for this copolymer may be written in the form
in which m_{b} and m_{s} are the repeat unit molecular weights for butadiene and styrene, respectively. These values are calculated as follows:
m_{b} = 4(A_{C}) + 6(A_{H}) = 4(12.01 g/mol) + 6(1.008 g/mol) = 54.09 g/mol
m_{s} = 8(A_{C}) + 8(A_{H}) = 8(12.01 g/mol) + 8(1.008 g/mol) = 104.14 g/mol
Solving for f_{b} in the above expression yields
Furthermore, f_{s} = 1 – f_{b} = 1 – 0.50 = 0.50; or the ratio is just
(b) Of the possible copolymers, the only one for which there is a restriction on the ratio of repeat unit types is alternating; the ratio must be 1:1. Therefore, on the basis of the result in part (a), the possibilities for this copolymer are not only alternating, but also random, graft, and block.
14.20 Crosslinked copolymers consisting of 60 wt% ethylene and 40 wt% propylene may have elastic properties similar to those for natural rubber. For a copolymer of this composition, determine the fraction of both repeat unit types.
Solution
For a copolymer consisting of 60 wt% ethylene and 40 wt% propylene, we are asked to determine the fraction of both repeat unit types.
In 100 g of this material, there are 60 g of ethylene and 40 g of propylene. The ethylene (C_{2}H_{4}) molecular weight is
m(ethylene) = 2(A_{C}) + 4(A_{H})
= (2)(12.01 g/mol) + (4)(1.008 g/mol) = 28.05 g/mol
The propylene (C_{3}H_{6}) molecular weight is
m(propylene) = 3(A_{C}) + 6(A_{H})
= (3)(12.01 g/mol) + (6)(1.008 g/mol) = 42.08 g/mol
Therefore, in 100 g of this material, there are
and
Thus, the fraction of the ethylene repeat unit, f(ethylene), is just
Likewise,
14.21 A random poly(isobutyleneisoprene) copolymer has a numberaverage molecular weight of 200,000 g/mol and a degree of polymerization of 3000. Compute the fraction of isobutylene and isoprene repeat units in this copolymer.
Solution
For a random poly(isobutyleneisoprene) copolymer in which = 200,000^{ }g/mol and DP = 3000, we are asked to compute the fractions of isobutylene and isoprene repeat units.
From Table 14.5, the isobutylene repeat unit has four carbon and eight hydrogen atoms. Thus,
m_{ib} = (4)(12.01 g/mol) + (8)(1.008 g/mol) = 56.10 g/mol
Also, from Table 14.5, the isoprene repeat unit has five carbon and eight hydrogen atoms, and
m_{ip} = (5)(12.01 g/mol) + (8)(1.008 g/mol) = 68.11 g/mol
From Equation 14.7
Now, let x = f_{ib}, such that
since f_{ib} + f_{ip} = 1. Also, from Equation 14.6
Or
Solving for x leads to x = f_{ib} = f(isobutylene) = 0.12. Also,
f(isoprene) = 1 – x = 1 – 0.12 = 0.88
Polymer Crystallinity
14.22 Explain briefly why the tendency of a polymer to crystallize decreases with increasing molecular weight.
Solution
The tendency of a polymer to crystallize decreases with increasing molecular weight because as the chains become longer it is more difficult for all regions along adjacent chains to align so as to produce the ordered atomic array.
14.23 For each of the following pairs of polymers, do the following: (1) state whether or not it is possible to determine whether one polymer is more likely to crystallize than the other; (2) if it is possible, note which is the more likely and then cite reason(s) for your choice; and (3) if it is not possible to decide, then state why.
(a) Linear and syndiotactic poly(vinyl chloride); linear and isotactic polystyrene.
(b) Network phenolformaldehyde; linear and heavily crosslinked cisisoprene.
(c) Linear polyethylene; lightly branched isotactic polypropylene.
(d) Alternating poly(styreneethylene) copolymer; random poly(vinyl chloridetetrafluoroethylene) copolymer.
Solution
(a) Yes, for these two polymers it is possible to decide. The linear and syndiotactic poly(vinyl chloride) is more likely to crystallize; the phenyl sidegroup for polystyrene is bulkier than the Cl sidegroup for poly(vinyl chloride). Syndiotactic and isotactic isomers are equally likely to crystallize.
(b) No, it is not possible to decide for these two polymers. Both heavily crosslinked and network polymers are not likely to crystallize.
(c) Yes, it is possible to decide for these two polymers. The linear polyethylene is more likely to crystallize. The repeat unit structure for polypropylene is chemically more complicated than is the repeat unit structure for polyethylene. Furthermore, branched structures are less likely to crystallize than are linear structures.
(d) Yes, it is possible to decide for these two copolymers. The alternating poly(styreneethylene) copolymer is more likely to crystallize. Alternating copolymers crystallize more easily than do random copolymers.
14.24 The density of totally crystalline polypropylene at room temperature is 0.946 g/cm^{3}. Also, at room temperature the unit cell for this material is monoclinic with lattice parameters
a = 0.666 nm α = 90
b = 2.078 nm β = 99.62
c = 0.650 nm γ = 90
If the volume of a monoclinic unit cell, V_{mono}, is a function of these lattice parameters as
V_{mono} = abc sin b
determine the number of repeat units per unit cell.
Solution
For this problem we are given the density of polypropylene (0.946 g/cm^{3}), an expression for the volume of its unit cell, and the lattice parameters, and are asked to determine the number of repeat units per unit cell. This computation necessitates the use of Equation 3.5, in which we solve for n. Before this can be carried out we must first calculate V_{C}, the unit cell volume, and A the repeat unit molecular weight. For V_{C}
V_{C} = abc sin b
= (0.666 nm)(2.078 nm)(0.650 nm) sin (99.62)
= 0.8869 nm^{3} = 8.869 10^{22} cm^{3}
The repeat unit for polypropylene is shown in Table 14.3, from which the value of A may be determined as follows:
A = 3(A_{C}) + 6(A_{H})
= 3(12.01 g/mol) + 6(1.008 g/mol)
= 42.08 g/mol
Finally, solving for n from Equation 3.5 leads to
= 12.0 repeat unit/unit cell
14.25 The density and associated percent crystallinity for two polytetrafluoroethylene materials are as follows:
ρ (g/cm^{3})

crystallinity (%)

2.144

51.3

2.215

74.2

(a) Compute the densities of totally crystalline and totally amorphous polytetrafluoroethylene.
(b) Determine the percent crystallinity of a specimen having a density of 2.26 g/cm^{3}.
Solution
(a) We are asked to compute the densities of totally crystalline and totally amorphous polytetrafluoroethylene (_{c} and _{a} from Equation 14.8). From Equation 14.8 let , such that
Rearrangement of this expression leads to
in which _{c} and _{a} are the variables for which solutions are to be found. Since two values of _{s} and C are specified in the problem statement, two equations may be constructed as follows:
In which _{s}_{1} = 2.144 g/cm^{3}, _{s}_{2} = 2.215 g/cm^{3},^{ }C_{1} = 0.513, and C_{2} = 0.742. Solving the above two equations for _{a} and _{c} leads to
And
(b) Now we are to determine the % crystallinity for _{s} = 2.26 g/cm^{3}. Again, using Equation 14.8
= 87.9%
14.26 The density and associated percent crystallinity for two nylon 6,6 materials are as follows:
ρ (g/cm^{3})

crystallinity (%)

1.188

67.3

1.152

43.7

(a) Compute the densities of totally crystalline and totally amorphous nylon 6,6.
(b) Determine the density of a specimen having 55.4% crystallinity.
Solution
(a) We are asked to compute the densities of totally crystalline and totally amorphous nylon 6,6 (_{c} and _{a} from Equation 14.8). From Equation 14.8 let , such that
Rearrangement of this expression leads to
in which _{c} and _{a} are the variables for which solutions are to be found. Since two values of _{s} and C are specified in the problem, two equations may be constructed as follows:
In which _{s}_{1} = 1.188 g/cm^{3}, _{s}_{2} = 1.152 g/cm^{3},^{ }C_{1} = 0.673, and C_{2} = 0.437. Solving the above two equations for _{a} and _{c} leads to
And
(b) Now we are asked to determine the density of a specimen having 55.4% crystallinity. Solving for _{s} from Equation 14.8 and substitution for _{a} and _{c} which were computed in part (a) yields
= 1.170 g/cm^{3}
Diffusion in Polymeric Materials
14.27 Consider the diffusion of water vapor through a polypropylene (PP) sheet 2 mm thick. The pressures of H_{2}O at the two faces are 1 kPa and 10 kPa, which are maintained constant. Assuming conditions of steady state, what is the diffusion flux [in [(cm^{3 }STP)/cm^{2}s] at 298 K?
Solution
This is a permeability problem in which we are asked to compute the diffusion flux of water vapor through a 2mm thick sheet of polypropylene. In order to solve this problem it is necessary to employ Equation 14.9. The permeability coefficient of H_{2}O through PP is given in Table 14.6 as 38 10^{13} (cm^{3} STP)cm/cm^{2}sPa. Thus, from Equation 14.9
and taking P_{1} = 1 kPa (1,000 Pa) and P_{2} = 10 kPa (10,000 Pa) we get
14.28 Argon diffuses through a high density polyethylene (HDPE) sheet 40 mm thick at a rate of 4.0 × 10^{–7 }(cm^{3 }STP)/cm^{2}s at 325 K. The pressures of argon at the two faces are 5000 kPa and 1500 kPa, which are maintained constant. Assuming conditions of steady state, what is the permeability coefficient at 325 K?
Solution
This problem asks us to compute the permeability coefficient for argon through high density polyethylene at 325 K given a steadystate permeability situation. It is necessary for us to Equation 14.9 in order to solve this problem. Rearranging this expression and solving for the permeability coefficient gives
Taking P_{1} = 1500 kPa (1,500,000 Pa) and P_{2} = 5000 kPa (5,000,000 Pa), the permeability coefficient of Ar through HDPE is equal to
14.29 The permeability coefficient of a type of small gas molecule in a polymer is dependent on absolute temperature according to the following equation:
where and Q_{p} are constants for a given gaspolymer pair. Consider the diffusion of hydrogen through a poly(dimethyl siloxane) (PDMSO) sheet 20 mm thick. The hydrogen pressures at the two faces are 10 kPa and 1 kPa, which are maintained constant. Compute the diffusion flux [in (cm^{3 }STP)/cm^{2 }–s]_{ }at 350 K. For this diffusion system
_{ }Q_{p} = 13.7 kJ/mol
Also, assume a condition of steady state diffusion
Solution
This problem asks that we compute the diffusion flux at 350 K for hydrogen in poly(dimethyl siloxane) (PDMSO). It is first necessary to compute the value of the permeability coefficient at 350 K. The temperature dependence of P_{M} is given in the problem statement, as follows:
And, incorporating values provided for the constants P_{M}_{0} and Q_{p}, we get
And, using Equation 14.9, the diffusion flux is equal to
Excerpts from this work may be reproduced by instructors for distribution on a notforprofit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
